Loading in 5 sec....

Stoner-Wohlfarth TheoryPowerPoint Presentation

Stoner-Wohlfarth Theory

- By
**lewis** - Follow User

- 225 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about ' Stoner-Wohlfarth Theory' - lewis

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

### Stoner-Wohlfarth Theory

“A Mechanism of Magnetic Hysteresis in Heterogenous Alloys”

Stoner E C and Wohlfarth E P (1948), Phil. Trans. Roy. Soc. A240:599–642

Prof. Bill Evenson, Utah Valley University

E.C. Stoner, c. 1934

E. C. Stoner, F.R.S.

and E. P. Wohlfarth (no

photo)

(Note:

F.R.S. = “Fellow of the Royal Society”)

Courtesy of AIP Emilio Segre Visual Archives

TU-Chemnitz

Stoner-Wohlfarth Motivation

- How to account for very high coercivities
- Domain wall motion cannot explain

- How to deal with small magnetic particles (e.g. grains or imbedded magnetic clusters in an alloy or mixture)
- Sufficiently small particles can only have a single domain

TU-Chemnitz

Domain Walls

- Weiss proposed the existence of magnetic domains in 1906-1907
- What elementary evidence suggests these structures?

www.cms.tuwien.ac.at/Nanoscience/Magnetism/magnetic-domains/magnetic_domains.htm

TU-Chemnitz

Stoner-Wohlfarth Problem

- Single domain particles (too small for domain walls)
- Magnetization of a particle is uniform and of constant magnitude
- Magnetization of a particle responds to external magnetic field and anisotropy energy

TU-Chemnitz

Not Stoner Theory of BandFerromagnetism

The Stoner-Wohlfarth theory of hysteresis does not refer to the Stoner (or Stoner-Slater) theory of band ferromagnetism or to such terms as “Stoner criterion”, “Stoner excitations”, etc.

TU-Chemnitz

Small magnetic particles

TU-Chemnitz

Why are we interested? (since 1948!)

Magnetic

nanostructures!

Can be single domain, uniform/constant magnetization, no long-range order between particles, anisotropic.

TU-Chemnitz

Physics in SW Theory

- Classical e & m (demagnetization fields, dipole)
- Weiss molecular field (exchange)
- Ellipsoidal particles for shape anisotropy
- Phenomenological magnetocrystalline and strain anisotropies
- Energy minimization

TU-Chemnitz

Outline of SW 1948 (1)

- 1. Introduction
- review of existing theories of domain wall motion (energy, process, effect of internal stress variations, effect of changing domain wall area – especially due to nonmagnetic inclusions)
- critique of boundary movement theory
- Alternative process: rotation of single domains (small magnetic particles – superparamagnetism) – roles of magneto-crystalline, strain, and shape anisotropies

TU-Chemnitz

Outline of SW 1948 (2)

- 2. Field Dependence of Magnetization Direction of a Uniformly Magnetized Ellipsoid – shape anisotropy
- 3. Computational Details
- 4. Prolate Spheroid Case
- 5. Oblate Spheroid and General Ellipsoid

TU-Chemnitz

Outline of SW 1948 (3)

- 6. Conditions for Single Domain Ellipsoidal Particles
- 7. Physical Implications
- types of magnetic anisotropy
- magnetocrystalline, strain, shape

- ferromagnetic materials
- metals & alloys containing FM impurities
- powder magnets
- high coercivity alloys

- types of magnetic anisotropy

TU-Chemnitz

Units, Terminology, Notation

E.g.

- Gaussian e-m units
- 1 Oe = 1000/4π × A/m

- Older terminology
- “interchange interaction energy” = “exchange interaction energy”

- Older notation
- I0 = magnetization vector

TU-Chemnitz

Mathematical Starting Point

- Applied field energy
- Anisotropy energy
- Total energy

(what should we use?)

(later, drop constants)

TU-Chemnitz

MAGNETIC ANISOTROPY

- Shape anisotropy (dipole interaction)
- Strain anisotropy
- Magnetocrystalline anisotropy
- Surface anisotropy
- Interface anisotropy
- Chemical ordering anisotropy
- Spin-orbit interaction
- Local structural anisotropy

TU-Chemnitz

Ellipsoidal particles

This gives shape anisotropy – from demagnetizing fields (to be discussed later if there is time).

Spherical particles would not have shape anisotropy, but would have magnetocrystalline and strain anisotropy – leading to the same physics with redefined parameters.

TU-Chemnitz

Ellipsoidal particles

We will look at one ellipsoidal particle, then average over a random orientation of particles.

The transverse components of mag-netization will cancel, and the net magnetiza-tion can be calculated as the component along the applied field direction.

TU-Chemnitz

Prolate and Oblate Spheroids

These show all the essential physics of the more general ellipsoid.

TU-Chemnitz

SW Fig. 1 – important notation

One can prove (SW outline the proof in Sec. 5(ii)) that for ellipsoids of revolution H, I0, and the easy axis all lie in

a plane.

TU-Chemnitz

Mathematical Starting Point - again

- Applied field energy
- Anisotropy energy
- Total energy

(later, drop constants)

TU-Chemnitz

Dimensionless variables

Total energy: normalize to and drop constant term.

Dimensionless energy is then

TU-Chemnitz

TU-Chemnitz

TU-Chemnitz

Examples in Maple

(This would be easy to do with Mathematica, also.)

[SW_Lectures_energy_surfaces.mw]

TU-Chemnitz

Calculating the Hysteresis Loop

TU-Chemnitz

TU-Chemnitz

TU-Chemnitz

Hsw and Hc

TU-Chemnitz

Average over Orientations

TU-Chemnitz

TU-Chemnitz

Part 2

- Conditions for large coercivity
- Applied field
- Various forms of magnetic anisotropy
- Conditions for single-domain ellipsoidal particles

TU-Chemnitz

Applied Field, H

- Important! This is the total field experienced by an individual particle.
It must include the field due to the magnetizations of all the other particles around the one we calculate!

TU-Chemnitz

Magnetic Anisotropy

- Regardless of the origin of the anisotropy energy, the basic physics is approximately the same as we have calculated for prolate spheroids.
- This is explicitly true for
- Shape anisotropy
- Magnetocrystalline anisotropy (uniaxial)
- Strain anisotropy

TU-Chemnitz

Demagnetizing Field Energy

- Energetics of magnetic media are very subtle.
is the “demagnetizing field”

from Blundell

TU-Chemnitz

How does depend on shape?

is extremely complicated for arbitrarily shaped ferromagnets, but relatively simple for ellipsoidal ones.

And in principal axis coordinate system for the ellipsoid,

TU-Chemnitz

Ferromagnet of Arbitrary Shape

TU-Chemnitz

Magnetocrystalline Anisotropy

- Uniaxial case is approximately the same mathematics as prolate spheroid. E.g. hexagonal cobalt:

For spherical, single domain particles of Co with easy axes oriented at random, coercivities ~2900 Oe. are possible.

TU-Chemnitz

Strain Anisotropy

- Uniaxial strain – again, approximately the same mathematics as prolate spheroid. E.g. magnetostriction coefficient λ, uniform tension σ:

TU-Chemnitz

Magnitudes of Anisotropies

- Prolate spheroids of Fe (m = a/b)
- shape > mc for m > 1.05
- shape > σ for m > 1.08

- Prolate spheroids of Ni
- shape > mc for m > 1.09
- σ > shape for all m (large λ, small I0)

- Prolate spheroids of Co
- shape > mc for m > 3
- shape > σ for m > 1.08

TU-Chemnitz

Conditions for Single Domain Ellipsoidal Particles

- Number of atoms must be
- large enough for ferromagnetic order within the particle
- small enough so that domain boundary formation is not energetically possible

TU-Chemnitz

Domain Walls (Bloch walls)

- Energies
- Exchange energy: costs energy to rotate neighboring spins
Rotation of N spins through total angle π, so , requires energy per unit area

- Anisotropy energy

- Exchange energy: costs energy to rotate neighboring spins

TU-Chemnitz

Domain Walls (2)

- Anisotropy energy:
magnetocrystalline

easy axis vs. hard axis

(from spin-orbit interaction and partial quenching of angular momentum)

shape

demagnetizing energy

It costs energy to rotate out of the easy

direction: say,

TU-Chemnitz

Conditions for Single Domain Ellipsoidal Particles (2)

- Demagnetizing field energy
- Uniform magnetization if ED < Ewall
- Fe: 105 – 106 atoms
- Ni: 107 – 1011 atoms

TU-Chemnitz

Thanks

- Friends at Uni-Konstanz, where this work was first carried out – some of this group are now at TU-Chemnitz
- Prof. Manfred Albrecht for invitation, hospitality and support

TU-Chemnitz

Download Presentation

Connecting to Server..